# Statistics Analysis Measures Painting of Cooling Tower

Authors: A. Zacharopoulou; E. Zacharopoulou; G. Batis
Journal: International Journal of Corrosion
 (2013)

---

## Abstract

This study refers to the cooling tower of Megalopolis (construction 1975) and protection from corrosive environment. The maintenance of the cooling tower took place in 2008. The cooling tower was badly damaged from corrosion of reinforcement. The parabolic cooling towers (factory of electrical power) are a typical example of construction, which has a special aggressive environment. The protection of cooling towers is usually achieved through organic coatings. Because of the different environmental impacts on the internal and external side of the cooling tower, a different system of paint application is required. The present study refers to the damages caused by corrosion process. The corrosive environments, the application of this painting, the quality control process, the measures and statistics analysis, and the results were discussed in this study. In the process of quality control the following measurements were taken into consideration: (1) examination of the adhesion with the cross-cut test, (2) examination of the film thickness, and (3) controlling of the pull-off resistance for concrete substrates and paintings. Finally, this study refers to the correlations of measurements, analysis of failures in relation to the quality of repair, and rehabilitation of the cooling tower. Also this study made a first attempt to apply the specific corrosion inhibitors in such a large structure.


---

## Body

## 1. Introduction

Generally the concrete comprises a protective environment of the reinforcement for the two reasons following.(i)
The aqueous solution of the pores of the reinforcement is intensely alkaline due to lime, which is the product of reaction of the cement hardening, its pH between 12.5 and 13.9. Under these circumstances, steel is superficially covered by a passive layer of iron oxides, which impedes its corrosion. Steel corrosion is restrictive to the maintenance of this passive layer; an action is so slow that it could practically be ignored.(ii)
The concrete acts as a natural barrier between the reinforcement and the various corrosive elements of the environment (such as oxygen and carbon dioxide) as well as other substances which may induce corrosion (such as chlorides).In time, cement may lose its protective capacity, for example, due to carbonation which is the reaction of carbon dioxide with calcium hydroxide. Then the pH may reach scales lower than 9, so the steel passes from the passive into the active state. Another reason for the corrosion of the reinforcement is the existence of chlorides. Chlorides penetrate the passive layer of oxides and cause corrosion in the form of acupuncture. The type of steel bars is S500s. The concrete coverage of rebar is 30 mm.The corrosion of the reinforcement into the concrete with pH lower than 9 is an electrochemical action, which takes place when three prerequisites are fulfilled:(i)
anodic dissolution of iron,(ii)
existence of oxygen,(iii)
electric conductivity through the pores of the cement.The speed of this action is highly dependent on the environmental conditions. It is quite slow in the case of the existence of the passive layer. However, it increases significantly when the pH value falls under 9. The same happens when the passive layer is destroyed by a sufficient amount of chlorides.Cooling towers are made of reinforced concrete. The reinforcement is like two nets, an interior, and an exterior one. Vertical reinforcements are placed on both the inner and the outer surface, towards the interior of the concrete while the horizontal ones are towards the exterior of concrete. As a consequence, vertical reinforcements are better protected against corrosion than the horizontal [1, 2].The corrosive environment on the inner side differs from the one on the outer [3, 4]. In the inside, the warm water introduced from the whirls of the production of electric current is inducted and then it is sprayed into plastic or wooden midriffs through a network of pipes. In this way, the water is evenly dispersed within the tower and part of it evaporates while the rest of it is cooled. The cool water is collected in the tank at the base of the cooling tower and then it is recycled. It is believed that inside the cooling tower (up to one particular height) there is only vapor and very little oxygen. The existence of oxygen into a higher point, through is significant. The vapor gets away from the top of the tower. On the inside surface of the tower a water membrane is formed. A portion of water from the inside of the cooling tower goes through the concrete and evaporates on the outer surface.The transfer of water creates the conductive environment which favors the corrosion of reinforcement in concrete. On the outside surface the influence of carbon dioxide is strong, because around the cooling tower was the chimney of turbines factory, which reduces the pH and oxygen and promotes creates of the oxides. Additionally it is mentioned that there are four additional power plants in the region around the cooling tower. Through this analysis, we conclude that on the outside surface of the tower signs of corrosion of the reinforcement are more likely to occur [5]. The inspection of the cooling tower verifies this theoretical picture (Figure 1).Figure 1
Cooling tower unit III of Megalopolis.The minimum and the maximum loss of existing reinforced section were from 0% to 70%. The use of cooling towers water to retain the sulfur oxide from the exhaust-gases changed the pH of water from neutral into acid. For this reason the protection of cooling towers must be strengthened.There were cases, as in Figure2 (thickness carbonation was 36 mm), that the depth of carbonation has overcome the concrete coverage.Figure 2
Ablation of concrete, before maintenance.


## 2. Corrosion and Deterioration of the Cooling Tower

Due to both operational and environmental conditions, the towers are liable to malfunctions because of the corrosion of the reinforcement. The cooling towers show many problems of corrosion of the reinforcement (Figure2). In this particular case, on the outside surface, in many places the reinforcement had been corroded and the cover of concrete was removed. At various points, the corrosion of reinforcement has reduced the diameter of rebar; therefore, the reinforcement must be cut and restored with new section of reinforcement. In this particular case, much attention was paid to the protection of reinforcements against corrosion and against carbonation in order to repair the tower [6, 7]. The applied method of protection against corrosion was the use of organic coatings. The requirements for the painting systems are explained in the instruction VGB “R 612 Ue” [8] (Protection Measures on Reinforced Concrete Cooling Towers and Chimneys against Operational and Environmental Impacts). Please note that the repair study was completed before application of EN1504.The method of repair provided the following.(i)
Removal of the covered parts of concrete to such an extent as to gain relevance of 1.5 MPa. In particular for the concrete of the inside surface of the cooling tower has to be the layer of organic deposits, which had been formed removed.(ii)
Cleaning of corroded reinforcement from corrosion products mechanically. Replacement reinforcement, which is necessary.(iii)
Coating of reinforcement with cementitious coatings.(iv)
Rehabilitation of concrete repair mortar.(v)
Protection of the cooling tower with an organic system coating on the surface of concrete.The purpose of the use of organic coatings is as follows.(i)
To prevent as much as possible the intrusion of water from the inside surface of the tower.(ii)
To help the outlet of the vapor on the outside surface, while at the same time reduce the inlet of oxygen and carbon dioxide.(iii)
In the case when the cooling tower is used to retain the waste-gases, the organic coating on the inside surface of the tower must be capable of enduring the acidity of the water.The system of organic coatings for the outside surface of the cooling tower was(1)
hydrophobic primer,(2)
two layers of acrylic emulsion of total thickness 200μm.The system of organic coatings for the inside surface of the cooling tower was(1)
epoxy primer,(2)
two layers of epoxy coating of total thickness 300μm (system 1),(3)
for the part of the interior of CT, existing solar radiation (above the ring) was covered with polyurethane 150μm (system 2).The final figure of the surface of the concrete after repair is shown in Figure3.Figure 3
Concrete after maintenance.


## 3. Measurement Methods

### 3.1. Controlling of the Pull-Off Test

Purpose of this method is to estimate the relevance of repair mortal concrete to the painting and to estimate the relevance of old concrete to the painting. According to BSEN 24624 (93) and ISO 4624 (1978) (Figure4).Figure 4
Pull-off test.


#### 3.1.1. Acceptance Measures

The testing of the pulloff was acceptable when the measures were better thanβΗΖ=1.5N/mm2. This value was chosen according to VGB “R 612 Ue.”


### 3.2. Examination of the Adhesion with the Cross-Cut Test

Purpose of this method is to estimate the adhesion of organic coating on the substrate and also between the primer and the second coating layer or between different coating layers or the cohesive strength of some substrates, according to ISO 2409N : 1992(E). The test is performed at temperature (23±2)°C, with special engraver made on the surface of the coating initially 6 horizontal alignments (20–30 mm) and then perpendicular to the previous 6 to form a lattice. All scratches must penetrate the surface of the substrate in accordance with the requirement of the standard. The test is performed at 3 different points; on the selected surface, where the 3 scores differ by more than one classification unit, the test should be repeated in another 3 points. The acceptance tests are the categories 0 and 1.


### 3.3. Measuring of the Film Thickness

The examination of the film thickness of the relevant surface protection coating shall be done with the wedge-cut test according to DIN 50986 [9]. Purpose of this method is to estimate the film thickness of concrete and also the film thickness of reinforcement (Figure 5).Figure 5
Cut test: measuring of the film thickness.


#### 3.3.1. Acceptance Measures

The minimum film thickness for reinforcement was acceptable:Smin=1000 μm.The minimum film thickness for concrete was acceptable:Smin=300 μm for system 1 and Smin=150 μm for system 2.Due to time constraints the project owner accepted that some areas of the cooling tower are to be recoated without measuring.


## 3.1. Controlling of the Pull-Off Test

Purpose of this method is to estimate the relevance of repair mortal concrete to the painting and to estimate the relevance of old concrete to the painting. According to BSEN 24624 (93) and ISO 4624 (1978) (Figure4).Figure 4
Pull-off test.


### 3.1.1. Acceptance Measures

The testing of the pulloff was acceptable when the measures were better thanβΗΖ=1.5N/mm2. This value was chosen according to VGB “R 612 Ue.”


## 3.1.1. Acceptance Measures

The testing of the pulloff was acceptable when the measures were better thanβΗΖ=1.5N/mm2. This value was chosen according to VGB “R 612 Ue.”


## 3.2. Examination of the Adhesion with the Cross-Cut Test

Purpose of this method is to estimate the adhesion of organic coating on the substrate and also between the primer and the second coating layer or between different coating layers or the cohesive strength of some substrates, according to ISO 2409N : 1992(E). The test is performed at temperature (23±2)°C, with special engraver made on the surface of the coating initially 6 horizontal alignments (20–30 mm) and then perpendicular to the previous 6 to form a lattice. All scratches must penetrate the surface of the substrate in accordance with the requirement of the standard. The test is performed at 3 different points; on the selected surface, where the 3 scores differ by more than one classification unit, the test should be repeated in another 3 points. The acceptance tests are the categories 0 and 1.


## 3.3. Measuring of the Film Thickness

The examination of the film thickness of the relevant surface protection coating shall be done with the wedge-cut test according to DIN 50986 [9]. Purpose of this method is to estimate the film thickness of concrete and also the film thickness of reinforcement (Figure 5).Figure 5
Cut test: measuring of the film thickness.


### 3.3.1. Acceptance Measures

The minimum film thickness for reinforcement was acceptable:Smin=1000 μm.The minimum film thickness for concrete was acceptable:Smin=300 μm for system 1 and Smin=150 μm for system 2.Due to time constraints the project owner accepted that some areas of the cooling tower are to be recoated without measuring.


## 3.3.1. Acceptance Measures

The minimum film thickness for reinforcement was acceptable:Smin=1000 μm.The minimum film thickness for concrete was acceptable:Smin=300 μm for system 1 and Smin=150 μm for system 2.Due to time constraints the project owner accepted that some areas of the cooling tower are to be recoated without measuring.


## 4. Experimental Part

The repair process begins with the removal of loose sections in order to achieve concrete strength above 1.5 MPa. Table1 shows the measurements of relevance that link the concrete with painting. Following the requirements of the study, the following measurements were obtained. All the values of the measurements are higher than the critical value of 1.5 MPa.Table 1
Measurements of pull-off test for external and internal shell.
External shell
Internal shell
Pull-off test
MPa
Pull-off test
MPa
1
3.1
1
3
2
3.9
2
3.5
3
2.1
3
2.8
4
2.4
4
3.2
5
2.4
5
2.7
6
1.6
6
1.8Then the removal of damaged reinforcement and the replacement with new reinforcement took place. Afterwards, the reinforcements are covered with cementitious coating.Figure6 shows the averages of measurements of the thickness of cementitious coating of reinforcement on the outside of the cooling tower. The axis X showed the separation areas of cooling tower. The average of measurements was not 1000 μm (according to the convention) but 850 μm.Figure 6
Thickness corrosion protection of rebar with cementitious coating for external shell.Figure7 shows the standard deviation of cementitious coating of reinforcement which was almost 195.23 μm in all working joints. The axis X showed the separation areas of cooling tower.Figure 7
Standard deviation of reinforcement of external shell.It should be noted that we faced certain difficulties when measuring the coating thickness of reinforcement:(1)
the surface of reinforcement is uneven. The height of nerves of reinforcement is 150μm;(2)
the back side of reinforcements (to concrete) is not suitable for uniform coating;(3)
the weather has an influence in the quality of work.From the above measurements we come to the conclusion that the difference between maximum and minimum value is 650μm. The overall distribution of coating thickness follows the normal distribution.Analytical measurements of Figures6 and 7 are presented in Table 2.Table 2
Thickness protection coating inμm of reinforcement for external shell.
Thickness corrosion protection reinforcement for external shell.
Working joints
Average
Min.
Max.
Standard deviation (SD)
Standard deviation (SD) (%)
6–12
967.24
567
1209
148.15
15.32
13–18
0
0
0
0
0
19–25
934.56
559
1209
159.40
17.06
26–31
670.48
220
1200
242.49
36.17
32–38
760.36
360
1100
235.47
30.97
39–45
725.41
209
1098
280.84
38.72
46–52
566.38
200
1095
228.05
40.26
53–58
778.09
222
1076
224.91
28.91
59–65
761.93
390
1153
232.38
30.50
63–68
683.32
258
986
232.34
34.00
66–71
964.65
699
1155
91.83
9.52
72–78
726.48
210
1078
217.90
29.99
79–85
740.64
420
1018
182.60
24.66
86–92
740.05
230
1158
264.87
35.79
93–98
737.73
366
1065
204.17
27.68
99–105
927.00
645
1153
116.03
12.52
105–111
699.55
245
993
251.71
35.98
112–117
747.37
346
1143
233.17
31.20
118–124
999.21
670
1342
144.84
14.50
125–131
1,000.05
651
1200
135.89
13.59
132–5
1,008.76
800
1217
105.78
10.49Figure8 shows the average measurements of the thickness of the anticorrosion coating of reinforcement on the inside of the cooling tower. It should be noted that the reinforcements, in general, were not covered with mortar repair. For the reinforcements above the ring of the cooling tower, the thickness of organic coatings had to be 950 μm (the thickness of cementitious coating 500 μm, the epoxy paint of concrete 300 μm, and polyurethane 150 μm). For the reinforcements under the ring of the cooling tower the thickness of paint had to be 800 μm. The average of values amounts to 875 μm. After applying the cement coating of reinforcement, it was followed by the application of mortar repair. After the restoration of concrete organic coatings were applied.Figure 8
Thickness protection coating of reinforcements (μm) for internal shell.Cementitious coating thickness of cooling tower reinforcements must be the same whether the reinforcement was located inside or outside of the cooling tower.Figure9 shows the standard deviation of measurements of the thickness of the anticorrosion coating of reinforcement on the inside of the cooling tower which was almost 223 μm in all working joints. The axis X showed the separation areas of cooling tower. Analytical measurements of Figures 8 and 9 are presented in Table 3.Table 3
Thickness corrosion protection inμm of reinforcement for internal shell.
Thickness corrosion protection reinforcement for external shell.
Working joints
Average
Min.
Max.
Standard deviation (SD)
Standard deviation (SD) (%)
6–12
856.05
600
1120
231.12
27.00
13–18
945.23
782
1105
210.95
22.32
19–25
959.73
750
1200
232.70
24.25
26–31
871.73
641
1150
231.91
26.60
32–38
866.68
670
1100
209.64
24.19
39–45
902.00
650
1100
222.97
24.72
46–52
892.52
700
1027
209.75
23.50
53–59
908.00
645
1090
208.77
23.88
60–66
971.76
680
1150
231.73
23.85
67–71
949.43
700
1180
221.89
23.37
72–77
955.71
780
1190
231.98
24.27
78–84
899.19
710
1032
208.61
23.20
85–91
899.00
637
1110
204.98
21.98
92–98
935.98
689
1150
216.34
22.96
99–104
890.87
700
1027
209.75
23.50
105–111
970.33
719
1190
256.98
20.99
112–118
928.05
690
1074
224.87
24.23
125–131
986.67
723
1200
241.94
24.52
132–5
948.38
730
1190
230.28
24.28Figure 9
Standard deviation of the total thickness coatings to concrete surface of the internal shell.The relevance of organic coatings of concrete was tested with the cross-cut method. The measurements are shown in Figure15 according to the ISO 2409N [10].The acceptance tests are the categories 0 and 1:category 0: none of the squares of the panel are detached;category 1: detachment of small flakes of coating on the prices of the lines affected an area of the panel not more than 5%.Figure10 shows the total coating thickness of acrylic coating on the outside of cooling tower. The thickness of the acrylic coating should be 200 μm. According to Figure 10, all measurements were greater than the limit (200 μm).Figure 10
Overall thickness paintings external shell.Figure11 shows the standard deviation and the standard deviation% of measurements of the coating outside of the cooling tower. The average standard deviation was almost 12.1 μm in all working joints. It is remarkable that the painting of concrete is simpler than the painting of reinforcement. Analytical measurements of Figures 10 and 11 are presented in Table 5.Figure 11
Standard deviation of acrylic emulsion coating on the surface of external shell.Figure12 shows the total coating thickness of organic coatings on the inside surface of the cooling tower. On the inside surface of the cooling tower two cases were presented (Table 6):(i)
under the ring of the cooling tower where the thickness of the coatings had to be 300μm epoxy paint,(ii)
above the ring of the cooling tower where the thickness of the coatings had to be 450μm (300 μm epoxy paint and 150 μm polyurethane).Figure 12
Total thickness of organic coatings (μm) on the surface of concrete internal shell (above the ring).Figure12 indicates that the average is 400 μm. Even the minimum values of measurements are over 350 μm.Figure13 shows the total coating standard deviation% and the standard deviation of organic coatings on the inside surface of the cooling tower. The average of standard deviation% was 10.59. Analytical measurements of Figures 12 and 13 are presented in Table 4.Table 4
Measurements of cross-cut for external and internal shell.
External shell
Internal shell
Relevance paintings
Category
Relevance paintings
Category
1
0
1
1
2
1
2
1
3
0
3
0
4
0
4
0
5
1
5
0
6
1
6
1Table 5
Total thickness of organic coatings (μm) on the concrete surface external shell under the ring.
Overall thickness paintings external  shell
Working joints
Average
Min.
Max.
Standard deviation (SD)
Standard deviation (SD) (%)
6–12
215.71
200
240
12.49
5.79
13–18
0
0
0
0
0
19–25
210.29
200
240
10.82
5.15
26–31
218.57
200
250
17.91
8.19
32–38
216.86
200
240
13.68
6.31
39–45
216.86
200
250
14.10
6.50
46–52
215.43
200
250
13.80
6.41
53–59
215.14
200
240
12.96
6.02
60–66
224.57
200
250
17.29
7.70
67–71
211.43
200
240
10.18
4.82
72–77
216.00
200
240
10.47
4.85
78–84
218.00
200
240
13.05
5.99
85–91
210.00
200
230
10.00
6.00
92–98
206.90
200
240
8.35
4.03
99–104
207.24
190
230
8.67
4.18
105–111
212.86
200
240
12.55
5.90
112–118
206.55
200
230
7.55
3.66
118–124
213.14
200
240
12.14
5.69
125–131
215.14
200
240
11.31
5.26
132–5
214.48
200
240
12.20
5.69Table 6
Organic coating total thickness (μm) on the surface concrete of internal shell (above the ring).
Overall thickness paintings internal shell
Working joints
Average
Min.
Max.
Standard deviation (SD)
Standard deviation (SD) (%)
6–12
398.33
300
500
80.709
20.26
13–18
490.83
480
510
10.961
2.23
19–25
480.00
450
520
22.361
4.66
26–31
390.56
300
480
72.147
18.47
32–38
440.42
310
540
80.324
18.24
39–45
527.22
500
580
25.507
4.84
46–52
387.22
300
490
72.786
18.80
53–59
478.33
460
500
16.750
3.50
60–66
461.67
340
510
60.702
13.15
67–71
403.33
300
490
71.880
17.82
72–77
480.00
440
530
22.870
4.97
78–84
470.00
450
520
23.805
5.06
85–91
481.11
450
510
18.526
3.85
92–98
401.11
300
485
72.102
17.98
99–104
498.33
480
520
12.134
2.43
105–111
387.06
300
480
80.130
20.70
112–118
475.00
450
500
17.078
3.60
125–131
418.00
300
490
73.230
17.52
132–5
477.78
450
510
15.476
3.24Figure 13
Overall standard deviation of paintings of internal shell (above the ring).Adhesion tests of organic coatings were also made using the pull-off method. These tests generally agree with the method cross-cut. In general, the adhesion of coatings on both arms and concrete was satisfactory despite the difficulties. The most difficult part of applying the coating was the weather, because of the intense humidity that existed in the atmosphere.After one year of operation, the cooling tower was shut down for three days to allow for the necessary maintenance works. Because of short time, it was not possible for measurements to be taken. During this time, an optical inspection of the internal tower was made, which showed good behavior of coatings. The reinforcements, which did not have mortar concrete, showed no general corrosion. As is evident from Figure11 (inner part), the state of epoxy coating is generally good and delamination and bubbles were not observed. The repair of concrete showed no problems. Red spots are corrosion products from the oxidation of protruding steels. This protruding steel is not reinforcement and exists only for the initial works. The protruding bars are covered only with epoxy primer.Figure14 shows that reinforcing bars, which protrude outward, are not part of the structure but simply exist only for supporting reasons.Figure 14
After a year of use of the cooling tower.Figure 15
Classification of the cross-cut test (standard ISO 2409: 1992 (E)).


## 5. Conclusions

The measurements of this study showed the following.(i)
The coverage of reinforcement with coating of cementations coating presented large fluctuations and the average of the measurements did not reach 1000μm.(ii)
The coverage of concrete with organic coatings, both internally and externally, reaches and exceeds the required limits.(iii)
The relevance of the coating with the substrate (reinforcement and concrete) was very good.(iv)
The average of the total thickness of coating on the outer shell is stable in all working joints but there was a great standard deviation.(v)
There was a greater standard deviation within the internal shell than in the outer shell. This is because there were more layers of painting inside (epoxy, polyurethane).



---

*Source: 389159-2013-12-16.xml*